- Home
- Documents
*MATERIALS OF CONSTRUCTION Introduction · MATERIALS OF CONSTRUCTION Introduction ... These...*

Click here to load reader

View

229Download

0

Embed Size (px)

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

1

MATERIALS OF CONSTRUCTION

Introduction

The engineering structures are composed of materials. These materials are known as

the engineering materials or building materials or materials of construction. It is

necessary for the civil engineer to become conversant with the properties of such

materials.

The service conditions of buildings demand a wide range of materials and various

properties such as water resistance, strength, durability, temperature resistance,

appearance, permeability, etc. are to be properly studied before making final

selection of any building material for a particular use.

Classification of Engineering material

The factors which form the basis of various systems of classifications of materials in

material science and engineering are: (i) the chemical composition of the material,

(ii) the mode of the occurrence of the material in the nature, (iii) the refining and the

manufacturing process to which the material is subjected prior it acquires the

required properties, (iv) the atomic and crystalline structure of material and (v) the

industrial and technical use of the material.

Common engineering materials that falls within the scope of material science and

engineering may beclassified into one of the following six groups:

(i) Metals (ferrous and non-ferrous) and alloys

(ii) Ceramics

(iii) Polymers

(iv) Composites

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

2

(vii) Advanced Materials

Properties of Engineering Materials

It is possible to classify material properties as follows :-

1- Physical properties:

Density, specific gravity, porosity, water absorption, etc ....

2- Mechanical properties:

Tensile strength, compressive strength, rigidity, hardness. Creep, fatigue ...... etc.

3- Thermal properties:

Thermal conductivity, thermal expansion and other .......

4- Chemical properties:

Resistance to acids, alkalis, brines and oxidation.

5- Economic characteristics:

Cost savings

6- Aesthetic properties:

Color, surface smoothness, the reflection of light

Physical properties

Density is defined as mass per unit volume for a material. The derived : ( Density

unit usually used by engineers is the kg/m3 . Relative density is the density of the

material compared with the density of the water at 4C.

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

3

The formula of density and relative density are:

Density of the material ( ) = M / V

Relative density (d) = Density of the material / Density of pure water at 4C

where;

M is material mass g, kg,etc

V is material volume m3, cm

3 ,etc

Density units : kg / m,gr / cm3, etc

There aretwotypesofdensity:

1- bulk density b: It is the ratio of material mass to total volume of material,

including spaces.

b = M / V

V = Vs + Vv

Vs = Volume of solids

Vv = volume of voids

V,M =total volume and total mass

Table (1) gives densities for some materials in kg/m3.

Materials Bulk density

(kg/m3)

Brick 1700

Mastic asphalt 2100

Cement:sand 2306

Glass 2520

Concrete 1:2:4 2260

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

4

Limestone 2310

Granite 2662

Steel 7850

Aluminum 2700

Copper 9000

lead 11340

Hardwoods 769

softwood, plywood 513

2-Solid density s

It is theratio of themassofsolidmaterialtothe volume ofsolidmaterialwithout any

spaces.

s = Ms / Vs

Unit weight

It is theratio of materialweight tomaterial volume.

= Unit weight (N / mm)

W= weight (N)

V = volume ( m)

= (M .g) / V = .g

is the specific weight of the material (weight per unit volume, typically N/m3

units)

is the density of the material (mass per unit volume, typically kg/m3)

http://en.wikipedia.org/wiki/Weighthttp://en.wikipedia.org/wiki/Volumehttp://en.wikipedia.org/wiki/Densityhttp://en.wikipedia.org/wiki/Masshttp://en.wikipedia.org/wiki/Volume

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

5

g is acceleration of gravity (rate of change of velocity, given in m/s2)

4- specific gravity( Gs)

A ratio of soliddensityof material anddensity ofdistilledwaterat a temperature of4co.

Gs = s /w

porosity (n)

It is the ratio of the volume of the spaces in the material to the over all volume.

Vv = Volume of voids

voids ratio (e)

It is theratiobetweenthesizeofvoidstothe volume ofsolidmaterial.

Water absorption

It denotes the ability of the material to absorb and retain water. It is

expressedaspercentage in weight or of the volume of dry material:

Ww =M1- M / M 100

Wv =M1 - M / V 100

where M1 = mass of saturated material (g)

M = mass of dry material (g)

V = volume of material including the pores (mm3)

Water absorption by volume is always less than 100 per cent, whereas that by

weight ofporous material may exceed 100 percent.

http://en.wikipedia.org/wiki/Standard_gravityhttp://en.wikipedia.org/wiki/Velocity

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

6

The properties of building materials are greatly influenced when saturated. The ratio

ofcompressive strength of material saturated with water to that in dry state is known

as coefficientof softening and describes the water resistance of materials. For

materials like clay which soakreadily it is zero, whereas for materials like glass and

metals it is one. Materials with coefficientof softening less than 0.8 should not be

recommended in the situations permanently exposedto the action of moisture.

Weathering resistance

It is the ability of a material to endure alternate wet and dry conditionsfor a long

period without considerable deformation and loss of mechanical strength.

Water permeability

It is the capacity of a material to allow water to penetrate under pressure.Materials

like glass, steel and bitumen are impervious.

Frost Resistance

It denotes the ability of a water-saturated material to endure repeated freezingand

thawing with considerable decrease of mechanical strength. Under such conditions

thewater contained by the pores increases in volume even up to 9 percent on

freezing.

Mechanical Properties

The properties which relate to material behavior under applied forces define as

mechanical properties. The common mechanical properties: Tensile strength,

compressive strength, rigidity, hardness. Creep, fatigue ...... etc.

- Strength is the ability of the material to resist failure under the action of stresses

caused by loads.

-Stress()is the applied force P divided by the original area Ao.

( = P / Ao).See Fig.1.

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

7

There are several types of stress which depend on types of applied load. These

stresses can be classified as:

1- Compression stress

2- Tension stress

3- Shear stress

4- Bending stress

5- Torsion stress

When bar is stretched, stresses are tensile (taken to be positive)

If forces are reversed, stresses are compressive (negative)

Fig.(1)Bar under tensile force

Example: Steel bar has a circular cross-section with diameter d = 50 mm and an

axial tensile load P = 10 kN. Find the normal stress.

Units are force per unit area = N / m2 = Pa (pascal). One Pa is very small, so we

usually work in MPa(mega-pascal, Pa x 106).

= 5.093MPa

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

8

Note that N / mm2 = MPa.

- Strain () is the change in length divided by the original length Lo ( = /

Lo). See Fig.1.

When bar is elongated, strains are tensile (positive).

When bar shortens, strains are compressive (negative).

Example:

Steel bar has length Lo = 2.0 m. A tensile load is applied which causes the bar to

extend by = 1.4 mm.

Find the normal strain.

The Poisson Effect

A positive (tensile) strain in one direction will also contribute a negative

(compressive) strain in the other direction, just as stretching a rubber band to make

it longer in one direction makes it thinner in the other directions (see Fig. 2). This

Greek letters

(delta)

(sigma)

(epsilon)

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

9

lateral contraction accompanying a longitudinal extension is called the Poisson

effect.

Figure (2) The Poisson Effect

So there is a tensile strain in the axial direction and a compressive strain in the other

two (lateral) directions.

The ratio of lateral strain of material to axial strain within elastic limit define as

Poissons ratio.

= (lateral strain/ axial strain)=(lateral/longitudinal)

Greek letter (nu)

The Poissons ratio is a dimensionless parameter that provides a good deal of insight

into the nature of the material. The major classes of engineered structural materials

fall neatly into order when ranked by Poissons ratio;

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

11

Example:

Two points fixed on steel bar of 10 mm diameter, the distance between points was

50 mm. tensile force applied on its ends (8 kN).The distance increased by 0.025 mm

and the diameter decreased by 0.0015 mm.

Determine:

1-Normal stress

2- Longitudinal and lateral strains

3- Poisson's ratio

A=

=78.57 mm2

= =

= 101.82 MPa

longitudinal= =

= 0.0005

lateral= =

0.0015=

= = = 0.3

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

11

Stress Strain Relationship

The relation between stress and strain is an extremely important measure of

amaterialsmechanicalproperties. Stress - strain curve is graphical representation of

it.

Stress-Strain Curve

1- The proportional limit

Up to the proportional limit for the material, the graph is a straight line and so the

stress is proportional to elastic strain and Hookes Law applies.

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

12

Proportional limit on Stress-Strain Curve

- Load is proportional to deformation .

- Stress is proportional to strain, material behaves elastically, There is no

permanent change to the material; when the load is removed, the material

resumes its original shape

- After the proportional limit, the graph changes from a straight Line

Hookes Law

Within the elastic region of the stress-strain diagram, stress is linearly proportional

to

strain (up to proportional limit).

- That relationship was formalized by Robert Hooke in 1678

- In mathematical terms Hooke's Law

= E

(sigma) is the axial/normal stress

E is the elastic modulus or the Youngs modulus

(epsilon) is the axial/normal strain

For shear stress in the same region Hooke's Law

= G

(tau) is the shear stress

G is the shear modulus or the modulus of rigidity

(gamma) is the shear strain

Modulus of Elasticity or Young's Modulus(E)

It is the slope of the initial linear portion of the stress-strain diagram. In other words

it is the ratio of stress to elastic strain.

E= /

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

13

The modulus of elasticity may also be characterized as the stiffness or ability of a

material to resist deformation within the linear range.

E (Steel) 200 x 103MPa

E (Aluminum) 70 x 103MPa

E (Concrete) 30 x 103MPa

Tangent Modulus (Et )

It is the slope of the stress-strain curve above the proportional limit. In other words

it is the ratio of stress to strain above the proportional limit. There is no single value

for the tangent modulus; it varies with strain.

Shear Modulus the modulus of rigidity (G)

It is the slope of the initial linear portion of the shear stress-strain diagram. In other

words it is the ratio of shear stress to elastic shear strain,

G= /

2- The Elastic Limit

It is the point after which the sample will notreturn to its original shape when the

load is released.

Elastic limit on stress strain curve

- The proportional limit and the elastic limit are very close. For most purposes,

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

14

we may consider them to be the same point.

- There is permanent change to the structure of the material.

3- Yield point

There may be a region of increased deformation without increased load

This point is known as the yield point. The stress at this point is called the yield

strength.

Yield point on stress strain curve

- After yield point, the material behaves plastically(when the load is removed,

the sample does not return to its original shape)

- It is not always easy to identify the yield point from the stress-strain (load-

deformation) curve. In these cases the offset method is used.

1- An offset for the material is given.

For the tension and compression labs, we use the following offsets:

For steel, use 0.2% strain

For brass, use 0.35% strain

For cast iron, use 0.05% strain

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

15

2- It is marked on the deformation (strain) axis.

3- A line through the offset point, parallel to the straight (proportional) part

of the curve,is drawn. The intersection of the line with the stress-strain

curve is taken to be the yield point.

offset method

4- The Strain-Hardening

After the yield point, there may be a region of where increased load is necessary for

increased deformation, This is the strain-hardening region

5- Ultimate strength

Load (stress) rises to a maximum; this is the ultimate strength of the material

6- Failure point

Load required for further deformation is reduced as the failure or breaking point is

approached.

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

16

Hardening strain, ultimate strength

and failure point on stress strain curve

Ductile and Brittle Materials

Each material has its own stress-strain curve, with different characteristics,

examples:

Glass (Brittle)

1- Ductile Material

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

17

Materials that are capable of undergoing large strains (at normal temperature)

before failure.

An advantage of ductile materials is that visible distortions may occur if the loads be

too large. Ductile materials are also capable of absorbing large amounts of energy

prior to failure.

Ductile materials include mild steel, aluminum and some of its alloys, copper,

magnesium, nickel, brass, bronze and many others.

2- Brittle Material

Materials that exhibit very little inelastic deformation. In other words, materials that

fail in tension at relatively low values of strain are considered brittle.

Brittle materials include concrete, stone, cast iron, glass and plaster.

Modulus of Elasticity Determination

Ductile Material, the modulus of elasticity is the slope of straight line of stress

strain curve.

E= /

Brittle materials, use one of followings:

1- Secant modulus

2- Initial tangent modulus

The slope of straight line between origin

point and point on curve has stress equal to

(2/3) of ultimate stress.

The tangent slope of stress-strain curve at

origin point.

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

18

3- Tangent modulus

Example

The following information obtained in tension test on a material as the sectional area

of the sample is 50 mm 2 and length 1000 mm, draw the stress - strain curve and

then determine the value of proportional limit , yield stress and ultimate strength,

failure stress and modulus of elasticity.

233 232 231 225 220 200 150 100 50 Load ( KN )

40 36 33 30 25 20 15 10 5 Extension ( mm )

225 240 275 290 300 295 275 250 238 Load ( KN )

160 150 136 120 100 80 60 50 45 Extension ( mm )

The tangent slope of stress-strain curve at

any point in elastic range, usually at yield

point.

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

19

Solution

Strain = /L

Extention

mm

Stress

=P/A

(MPa)

Load, P

(kN)

0 0 0 0

0.005 5 100 50

0.01 10 200 100

0.015 15 300 150

0.02 20 400 200

0.025 25 440 220

0.03 30 450 225

0.033 33 462 231

0.036 36 464 232

0.04 40 466 233

0.045 45 476 238

0.05 50 500 250

0.06 60 550 275

0.08 80 590 295

0.1 100 600 300

0.12 120 580 290

0.136 136 550 275

0.15 150 480 240

0.16 160 450 225

Example

The following information obtained in compression test on concrete cylinder, draw

the stress - strain curve and then determine ultimate compressive strength

15 20 51 51 1 1 Stress (MPa)

21 15 9 5 2 1 Strain x10-4

Civil Engineering Department Materials of Construction

NOTES:

lecturer: Dr. Sa'adFahadResan

21